data_njy1
_audit_creation_date              2016-10-28
_audit_creation_method
;
Olex2 1.2-beta
(compiled 2015.01.26 svn.r3150 for OlexSys, GUI svn.r4998)
;
_publ_contact_author_address      ?
_publ_contact_author_email        ?
_publ_contact_author_name         ''
_publ_contact_author_phone        ?
_publ_section_references
;
Dolomanov, O.V., Bourhis, L.J., Gildea, R.J, Howard, J.A.K. & Puschmann, H.
 (2009), J. Appl. Cryst. 42, 339-341.

Sheldrick, G.M. (2008). Acta Cryst. A64, 112-122.
;
_chemical_name_common             ?
_chemical_name_systematic         ?
_chemical_formula_moiety          '0.25(K24 Na16 O1488 Tb48 W348), 38(O)'
_chemical_formula_sum             'H172 K6 Na4 O410 Tb12 W87'
_chemical_formula_weight          24961.92
_chemical_absolute_configuration  ?
_chemical_melting_point           ?
loop_
  _atom_type_symbol
  _atom_type_description
  _atom_type_scat_dispersion_real
  _atom_type_scat_dispersion_imag
  _atom_type_scat_source
 'C' 'C' 0.0033 0.0016 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
 'H' 'H' 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
 'Na' 'Na' 0.0362 0.0249 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
 'O' 'O' 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
 'P' 'P' 0.1023 0.0942 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
 'Nb' 'Nb' -2.0727 0.6215
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
 'Tb' 'Tb' -0.1723 4.1537
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
 'W' 'W' -0.8490 6.8722 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
 'K' 'K' 0.2009 0.2494 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'

_shelx_space_group_comment
;
The symmetry employed for this shelxl refinement is uniquely defined
by the following loop, which should always be used as a source of
symmetry information in preference to the above space-group names.
They are only intended as comments.
;
_space_group_crystal_system       'cubic'
_space_group_IT_number            220
_space_group_name_H-M_alt         'I -4 3 d'
_space_group_name_Hall            'I -4bd 2c 3'
loop_
  _space_group_symop_operation_xyz
 'x, y, z'
 '-x+1/2, -y, z+1/2'
 '-x, y+1/2, -z+1/2'
 'x+1/2, -y+1/2, -z'
 'z, x, y'
 'z+1/2, -x+1/2, -y'
 '-z+1/2, -x, y+1/2'
 '-z, x+1/2, -y+1/2'
 'y, z, x'
 '-y, z+1/2, -x+1/2'
 'y+1/2, -z+1/2, -x'
 '-y+1/2, -z, x+1/2'
 'y+1/4, x+1/4, z+1/4'
 '-y+1/4, -x+3/4, z+3/4'
 'y+3/4, -x+1/4, -z+3/4'
 '-y+3/4, x+3/4, -z+1/4'
 'x+1/4, z+1/4, y+1/4'
 '-x+3/4, z+3/4, -y+1/4'
 '-x+1/4, -z+3/4, y+3/4'
 'x+3/4, -z+1/4, -y+3/4'
 'z+1/4, y+1/4, x+1/4'
 'z+3/4, -y+1/4, -x+3/4'
 '-z+3/4, y+3/4, -x+1/4'
 '-z+1/4, -y+3/4, x+3/4'
 'x+1/2, y+1/2, z+1/2'
 '-x+1, -y+1/2, z+1'
 '-x+1/2, y+1, -z+1'
 'x+1, -y+1, -z+1/2'
 'z+1/2, x+1/2, y+1/2'
 'z+1, -x+1, -y+1/2'
 '-z+1, -x+1/2, y+1'
 '-z+1/2, x+1, -y+1'
 'y+1/2, z+1/2, x+1/2'
 '-y+1/2, z+1, -x+1'
 'y+1, -z+1, -x+1/2'
 '-y+1, -z+1/2, x+1'
 'y+3/4, x+3/4, z+3/4'
 '-y+3/4, -x+5/4, z+5/4'
 'y+5/4, -x+3/4, -z+5/4'
 '-y+5/4, x+5/4, -z+3/4'
 'x+3/4, z+3/4, y+3/4'
 '-x+5/4, z+5/4, -y+3/4'
 '-x+3/4, -z+5/4, y+5/4'
 'x+5/4, -z+3/4, -y+5/4'
 'z+3/4, y+3/4, x+3/4'
 'z+5/4, -y+3/4, -x+5/4'
 '-z+5/4, y+5/4, -x+3/4'
 '-z+3/4, -y+5/4, x+5/4'

_cell_length_a                    35.774(4)
_cell_length_b                    35.774(4)
_cell_length_c                    35.774(4)
_cell_angle_alpha                 90
_cell_angle_beta                  90
_cell_angle_gamma                 90
_cell_volume                      45784(16)
_cell_formula_units_Z             4
_cell_measurement_reflns_used     1070
_cell_measurement_temperature     296(2)
_cell_measurement_theta_max       16.02
_cell_measurement_theta_min       2.55
_shelx_estimated_absorpt_T_max    0.070
_shelx_estimated_absorpt_T_min    0.033
_exptl_absorpt_coefficient_mu     23.739
_exptl_absorpt_correction_T_max   0.0697
_exptl_absorpt_correction_T_min   0.0332
_exptl_absorpt_correction_type    'Multi-scan'
_exptl_absorpt_process_details    SADABS
_exptl_absorpt_special_details    ?
_exptl_crystal_colour             colorless
_exptl_crystal_density_diffrn     3.621
_exptl_crystal_density_meas       .
_exptl_crystal_density_method     ?
_exptl_crystal_description        block
_exptl_crystal_F_000              43312
_exptl_crystal_size_max           0.45
_exptl_crystal_size_mid           0.31
_exptl_crystal_size_min           0.24
_exptl_transmission_factor_max    ?
_exptl_transmission_factor_min    ?
_diffrn_reflns_av_R_equivalents   0.1012
_diffrn_reflns_av_unetI/netI      0.0418
_diffrn_reflns_Laue_measured_fraction_full 0.996
_diffrn_reflns_Laue_measured_fraction_max 0.996
_diffrn_reflns_limit_h_max        42
_diffrn_reflns_limit_h_min        -42
_diffrn_reflns_limit_k_max        42
_diffrn_reflns_limit_k_min        -42
_diffrn_reflns_limit_l_max        42
_diffrn_reflns_limit_l_min        -22
_diffrn_reflns_number             113413
_diffrn_reflns_point_group_measured_fraction_full 0.997
_diffrn_reflns_point_group_measured_fraction_max 0.997
_diffrn_reflns_theta_full         25.088
_diffrn_reflns_theta_max          25.088
_diffrn_reflns_theta_min          1.610
_diffrn_ambient_temperature       296.15
_diffrn_detector_area_resol_mean  ?
_diffrn_measured_fraction_theta_full 0.996
_diffrn_measured_fraction_theta_max 0.996
_diffrn_measurement_device_type   'CCD area detector'
_diffrn_measurement_method        'phi and omega scans'
_diffrn_radiation_monochromator   'graphite'
_diffrn_radiation_type            MoK\a
_diffrn_radiation_wavelength      0.71073
_diffrn_source                    ?
_reflns_Friedel_coverage          0.902
_reflns_Friedel_fraction_full     0.998
_reflns_Friedel_fraction_max      0.998
_reflns_number_gt                 5972
_reflns_number_total              6779
_reflns_special_details
;
 Reflections were merged by SHELXL according to the crystal
 class for the calculation of statistics and refinement.
 
 _reflns_Friedel_fraction is defined as the number of unique
 Friedel pairs measured divided by the number that would be
 possible theoretically, ignoring centric projections and
 systematic absences.
;
_reflns_threshold_expression      'I > 2σ(I)'
_computing_cell_refinement        'SAINT v7.34A (Bruker, 200?)'
_computing_data_collection        ?
_computing_data_reduction         'SAINT v7.34A (Bruker, 200?)'
_computing_molecular_graphics     'Olex2 (Dolomanov et al., 2009)'
_computing_publication_material   'Olex2 (Dolomanov et al., 2009)'
_computing_structure_refinement   'ShelXL-2014/7 (Sheldrick, 2008)'
_computing_structure_solution     'ShelXS-1997 (Sheldrick, 2008)'
_refine_diff_density_max          1.630
_refine_diff_density_min          -1.378
_refine_diff_density_rms          0.278
_refine_ls_abs_structure_details
;
 Flack x determined using 2681 quotients [(I+)-(I-)]/[(I+)+(I-)]
 (Parsons, Flack and Wagner, Acta Cryst. B69 (2013) 249-259).
;
_refine_ls_abs_structure_Flack    -0.046(10)
_refine_ls_extinction_coef        .
_refine_ls_extinction_method      none
_refine_ls_goodness_of_fit_ref    1.187
_refine_ls_hydrogen_treatment     undef
_refine_ls_matrix_type            full
_refine_ls_number_parameters      406
_refine_ls_number_reflns          6779
_refine_ls_number_restraints      78
_refine_ls_R_factor_all           0.0520
_refine_ls_R_factor_gt            0.0352
_refine_ls_restrained_S_all       1.188
_refine_ls_shift/su_max           0.001
_refine_ls_shift/su_mean          0.000
_refine_ls_structure_factor_coef  Fsqd
_refine_ls_weighting_details
'w=1/[σ²(Fo²)+(0.0298P)²+2211.5415P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme       calc
_refine_ls_wR_factor_gt           0.0790
_refine_ls_wR_factor_ref          0.0925
_refine_special_details           ?
_olex2_refinement_description
;
1. Uiso/Uaniso restraints and constraints
Uanis(O1W) \\sim Ueq, Uanis(O4W) \\sim Ueq, Uanis(O27) \\sim Ueq, Uanis(O16)
\\sim Ueq: with sigma of 0.01 and sigma for terminal atoms of 0.02
Uanis(O7W) \\sim Ueq, Uanis(O10W) \\sim Ueq, Uanis(O19) \\sim Ueq, Uanis(O22)
\\sim Ueq, Uanis(O8W) \\sim Ueq: with sigma of 0.01 and sigma for terminal
atoms of 0.02
Uanis(O5W) \\sim Ueq, Uanis(O1) \\sim Ueq, Uanis(O20) \\sim Ueq: with sigma of
0.005 and sigma for terminal atoms of 0.01
Uanis(O9W) \\sim Ueq: with sigma of 0.02 and sigma for terminal atoms of 0.04
2. Others
 Fixed Sof: O7W(0.5) O8W(0.5) O9W(0.16667) O10W(0.5)
;
_atom_sites_solution_hydrogens    .
_atom_sites_solution_primary      direct
_atom_sites_solution_secondary    ?
loop_
  _atom_site_label
  _atom_site_type_symbol
  _atom_site_fract_x
  _atom_site_fract_y
  _atom_site_fract_z
  _atom_site_U_iso_or_equiv
  _atom_site_adp_type
  _atom_site_occupancy
  _atom_site_site_symmetry_order
  _atom_site_calc_flag
  _atom_site_refinement_flags_posn
  _atom_site_refinement_flags_adp
  _atom_site_refinement_flags_occupancy
  _atom_site_disorder_assembly
  _atom_site_disorder_group
 W1 W 0.5000 0.2500 0.1250 0.0110(4) Uani 1 4 d S T P . .
 W2 W 0.54619(3) 0.15140(3) 0.06755(3) 0.0163(2) Uani 1 1 d . . . . .
 W3 W 0.60208(3) 0.22278(3) 0.06522(3) 0.0162(2) Uani 1 1 d . . . . .
 W4 W 0.61277(3) 0.15421(3) -0.00047(3) 0.0253(3) Uani 1 1 d . . . . .
 W5 W 0.54939(4) 0.08713(3) 0.00445(3) 0.0307(3) Uani 1 1 d . . . . .
 W6 W 0.53131(4) 0.15660(4) -0.05088(3) 0.0335(3) Uani 1 1 d . . . . .
 W7 W 0.58683(4) 0.22902(4) -0.05476(3) 0.0378(3) Uani 1 1 d . . . . .
 W8 W 0.66036(4) 0.23346(4) -0.00207(4) 0.0366(3) Uani 1 1 d . . . . .
 Tb1 Tb 0.58147(3) 0.18387(3) 0.16894(4) 0.0192(3) Uani 1 1 d . . . . .
 K1 K 0.5000 0.2500 0.0203(3) 0.037(2) Uani 1 2 d S T P . .
 Na1 Na 0.5099(5) -0.0099(5) 0.0099(5) 0.063(8) Uani 1 3 d S T P . .
 O1 O 0.5322(4) 0.2243(4) 0.1531(5) 0.016(3) Uani 1 1 d . U . . .
 O2 O 0.5579(5) 0.1512(5) 0.1151(5) 0.022(4) Uani 1 1 d . . . . .
 O3 O 0.4975(5) 0.1498(5) 0.0645(5) 0.022(4) Uani 1 1 d . . . . .
 O4 O 0.5512(5) 0.2052(5) 0.0592(5) 0.023(4) Uani 1 1 d . . . . .
 O5 O 0.6055(5) 0.1622(5) 0.0514(5) 0.023(4) Uani 1 1 d . . . . .
 O6 O 0.5582(5) 0.1007(5) 0.0571(5) 0.026(4) Uani 1 1 d . . . . .
 O7 O 0.5512(5) 0.1457(5) 0.0070(5) 0.028(4) Uani 1 1 d . . . . .
 O8 O 0.6077(5) 0.2124(5) 0.1131(5) 0.024(4) Uani 1 1 d . . . . .
 O9 O 0.5926(5) 0.2709(5) 0.0622(5) 0.025(4) Uani 1 1 d . . . . .
 O10 O 0.6536(5) 0.2219(5) 0.0516(6) 0.031(5) Uani 1 1 d . . . . .
 O11 O 0.6052(5) 0.2167(5) 0.0042(5) 0.025(4) Uani 1 1 d . . . . .
 O12 O 0.6118(5) 0.1041(5) -0.0025(6) 0.036(5) Uani 1 1 d . . . . .
 O13 O 0.6602(5) 0.1667(6) -0.0062(5) 0.032(5) Uani 1 1 d . . . . .
 O14 O 0.5931(5) 0.1661(6) -0.0481(5) 0.030(5) Uani 1 1 d . . . . .
 O15 O 0.5020(6) 0.0791(6) 0.0111(6) 0.037(5) Uani 1 1 d . . . . .
 O16 O 0.5459(6) 0.1041(6) -0.0476(5) 0.037(5) Uani 1 1 d . U . . .
 O17 O 0.5713(6) 0.0403(6) 0.0204(7) 0.050(6) Uani 1 1 d . . . . .
 O18 O 0.5650(8) 0.0417(7) -0.0181(7) 0.058(7) Uani 1 1 d . . . . .
 O19 O 0.4844(5) 0.1510(7) -0.0381(5) 0.041(6) Uani 1 1 d . U . . .
 O20 O 0.5317(7) 0.1583(7) -0.0996(6) 0.048(6) Uani 1 1 d . U . . .
 O21 O 0.5387(6) 0.2089(6) -0.0394(6) 0.043(6) Uani 1 1 d . . . . .
 O22 O 0.5825(7) 0.2274(7) -0.1030(6) 0.051(6) Uani 1 1 d . U . . .
 O23 O 0.5771(8) 0.2753(6) -0.0436(7) 0.055(7) Uani 1 1 d . . . . .
 O24 O 0.6416(6) 0.2289(7) -0.0532(6) 0.045(6) Uani 1 1 d . . . . .
 O25 O 0.6566(7) 0.2809(6) 0.0014(7) 0.054(7) Uani 1 1 d . . . . .
 O26 O 0.7074(7) 0.2297(9) -0.0283(9) 0.069(8) Uani 1 1 d . . . . .
 O27 O 0.7121(7) 0.2259(7) 0.0119(8) 0.058(7) Uani 1 1 d . U . . .
 O1W O 0.6355(7) 0.1418(7) 0.1402(7) 0.060(7) Uani 1 1 d . U . . .
 O2W O 0.5856(6) 0.1213(7) 0.1988(7) 0.051(6) Uani 1 1 d . . . . .
 O3W O 0.5631(6) 0.1983(7) 0.2331(6) 0.044(6) Uani 1 1 d . . . . .
 O4W O 0.6422(7) 0.1886(7) 0.2023(8) 0.066(8) Uani 1 1 d . U . . .
 O5W O 0.6906(6) 0.2026(7) 0.1192(6) 0.047(6) Uani 1 1 d . U . . .
 O6W O 0.7500 0.2935(10) 0.0000 0.084(15) Uani 1 2 d S T P . .
 O7W O 0.4315(13) 0.1652(13) -0.0960(11) 0.048(12) Uani 0.5 1 d . U . . .
 O8W O 0.5869(12) 0.0693(10) 0.1265(11) 0.032(9) Uani 0.5 1 d . U . . .
 O9W O 0.450(2) 0.050(2) -0.050(2) 0.12(4) Uani 0.5 3 d S TU P . .
 O10W O 0.697(2) 0.158(2) 0.072(2) 0.10(2) Uani 0.5 1 d . U . . .


_geom_special_details
;
 All esds (except the esd in the dihedral angle between two l.s. planes)
 are estimated using the full covariance matrix.  The cell esds are taken
 into account individually in the estimation of esds in distances, angles
 and torsion angles; correlations between esds in cell parameters are only
 used when they are defined by crystal symmetry.  An approximate (isotropic)
 treatment of cell esds is used for estimating esds involving l.s. planes.
;
loop_
  _geom_bond_atom_site_label_1
  _geom_bond_atom_site_label_2
  _geom_bond_distance
  _geom_bond_site_symmetry_2
  _geom_bond_publ_flag
 W1 K1 3.747(10) . ?
 W1 K1 3.747(10) 39_454 ?
 W1 O1 1.786(15) . ?
 W1 O1 1.786(15) 16_545 ?
 W1 O1 1.786(15) 39_454 ?
 W1 O1 1.786(15) 26_554 ?
 W2 W5 3.2242(15) . ?
 W2 O2 1.752(17) . ?
 W2 O3 1.747(17) . ?
 W2 O4 1.955(19) . ?
 W2 O5 2.232(18) . ?
 W2 O6 1.902(17) . ?
 W2 O7 2.182(19) . ?
 W3 W8 3.2073(16) . ?
 W3 K1 4.108(4) . ?
 W3 O4 1.937(17) . ?
 W3 O5 2.226(18) . ?
 W3 O8 1.763(18) . ?
 W3 O9 1.760(16) . ?
 W3 O10 1.906(17) . ?
 W3 O11 2.195(19) . ?
 W4 O5 1.896(18) . ?
 W4 O7 2.240(18) . ?
 W4 O11 2.259(17) . ?
 W4 O12 1.795(19) . ?
 W4 O13 1.767(18) . ?
 W4 O14 1.894(18) . ?
 W5 O6 1.969(17) . ?
 W5 O7 2.099(18) . ?
 W5 O12 2.33(2) . ?
 W5 O15 1.74(2) . ?
 W5 O16 1.96(2) . ?
 W5 O17 1.94(2) . ?
 W5 O18 1.90(2) . ?
 W6 O7 2.22(2) . ?
 W6 O14 2.24(2) . ?
 W6 O16 1.95(2) . ?
 W6 O19 1.75(2) . ?
 W6 O20 1.74(2) . ?
 W6 O21 1.93(2) . ?
 W7 O11 2.254(19) . ?
 W7 O14 2.27(2) . ?
 W7 O21 1.94(2) . ?
 W7 O22 1.73(2) . ?
 W7 O23 1.74(2) . ?
 W7 O24 1.96(2) . ?
 W8 O10 1.98(2) . ?
 W8 O11 2.074(18) . ?
 W8 O13 2.39(2) . ?
 W8 O24 1.96(2) . ?
 W8 O25 1.71(2) . ?
 W8 O26 1.93(2) . ?
 W8 O27 1.93(3) . ?
 Tb1 K1 4.338(5) 39_454 ?
 Tb1 O1 2.348(15) . ?
 Tb1 O2 2.406(16) . ?
 Tb1 O3 2.444(16) 16_545 ?
 Tb1 O8 2.432(19) . ?
 Tb1 O9 2.457(16) 39_454 ?
 Tb1 O1W 2.66(2) . ?
 Tb1 O2W 2.48(2) . ?
 Tb1 O3W 2.44(2) . ?
 Tb1 O4W 2.48(2) . ?
 K1 W3 4.108(4) 26_554 ?
 K1 Tb1 4.339(5) 16_545 ?
 K1 O1 3.112(19) 39_454 ?
 K1 O1 3.112(19) 16_545 ?
 K1 O4 2.805(18) . ?
 K1 O4 2.805(18) 26_554 ?
 K1 O21 2.94(2) 26_554 ?
 K1 O21 2.94(2) . ?
 K1 O3W 2.92(2) 39_454 ?
 K1 O3W 2.92(2) 16_545 ?
 Na1 O17 2.86(2) 6 ?
 Na1 O17 2.86(2) . ?
 Na1 O17 2.86(2) 12_554 ?
 Na1 O18 2.88(3) 6 ?
 Na1 O18 2.88(3) 12_554 ?
 Na1 O18 2.88(3) . ?
 O1 K1 3.112(19) 39_454 ?
 O3 Tb1 2.444(16) 39_454 ?
 O9 Tb1 2.457(16) 16_545 ?
 O17 O18 1.40(3) . ?
 O26 O27 1.45(4) . ?
 O3W K1 2.92(2) 39_454 ?

loop_
  _geom_angle_atom_site_label_1
  _geom_angle_atom_site_label_2
  _geom_angle_atom_site_label_3
  _geom_angle
  _geom_angle_site_symmetry_1
  _geom_angle_site_symmetry_3
  _geom_angle_publ_flag
 K1 W1 K1 180.0 39_454 . ?
 O1 W1 K1 55.7(5) 16_545 . ?
 O1 W1 K1 55.7(5) . 39_454 ?
 O1 W1 K1 55.7(5) 39_454 . ?
 O1 W1 K1 124.3(5) . . ?
 O1 W1 K1 124.3(5) 39_454 39_454 ?
 O1 W1 K1 124.3(5) 26_554 . ?
 O1 W1 K1 124.3(5) 16_545 39_454 ?
 O1 W1 K1 55.7(5) 26_554 39_454 ?
 O1 W1 O1 108.5(5) 39_454 26_554 ?
 O1 W1 O1 108.5(5) 16_545 26_554 ?
 O1 W1 O1 111.4(11) 26_554 . ?
 O1 W1 O1 111.4(11) 39_454 16_545 ?
 O1 W1 O1 108.5(5) 16_545 . ?
 O1 W1 O1 108.5(5) 39_454 . ?
 O2 W2 W5 132.0(6) . . ?
 O2 W2 O4 97.5(8) . . ?
 O2 W2 O5 91.5(7) . . ?
 O2 W2 O6 97.7(8) . . ?
 O2 W2 O7 160.7(8) . . ?
 O3 W2 W5 88.2(6) . . ?
 O3 W2 O2 107.3(8) . . ?
 O3 W2 O4 96.6(8) . . ?
 O3 W2 O5 159.7(7) . . ?
 O3 W2 O6 100.5(8) . . ?
 O3 W2 O7 91.0(8) . . ?
 O4 W2 W5 126.2(5) . . ?
 O4 W2 O5 72.7(7) . . ?
 O4 W2 O7 86.1(7) . . ?
 O5 W2 W5 84.8(5) . . ?
 O6 W2 W5 34.3(5) . . ?
 O6 W2 O4 152.5(8) . . ?
 O6 W2 O5 84.2(7) . . ?
 O6 W2 O7 72.3(7) . . ?
 O7 W2 W5 40.2(5) . . ?
 O7 W2 O5 71.4(7) . . ?
 W8 W3 K1 104.82(12) . . ?
 O4 W3 W8 124.4(5) . . ?
 O4 W3 K1 36.7(5) . . ?
 O4 W3 O5 73.1(7) . . ?
 O4 W3 O11 84.5(7) . . ?
 O5 W3 W8 85.1(5) . . ?
 O5 W3 K1 101.1(4) . . ?
 O8 W3 W8 132.9(6) . . ?
 O8 W3 K1 122.0(6) . . ?
 O8 W3 O4 98.4(8) . . ?
 O8 W3 O5 90.3(7) . . ?
 O8 W3 O10 97.8(9) . . ?
 O8 W3 O11 159.8(7) . . ?
 O9 W3 W8 87.9(6) . . ?
 O9 W3 K1 64.6(6) . . ?
 O9 W3 O4 97.4(8) . . ?
 O9 W3 O5 161.8(8) . . ?
 O9 W3 O8 106.7(9) . . ?
 O9 W3 O10 100.8(8) . . ?
 O9 W3 O11 92.6(8) . . ?
 O10 W3 W8 35.1(6) . . ?
 O10 W3 K1 139.7(7) . . ?
 O10 W3 O4 150.9(8) . . ?
 O10 W3 O5 82.8(8) . . ?
 O10 W3 O11 72.2(8) . . ?
 O11 W3 W8 39.9(5) . . ?
 O11 W3 K1 71.3(5) . . ?
 O11 W3 O5 71.4(6) . . ?
 O5 W4 O7 76.6(7) . . ?
 O5 W4 O11 76.2(7) . . ?
 O7 W4 O11 90.5(7) . . ?
 O12 W4 O5 100.8(9) . . ?
 O12 W4 O7 81.4(8) . . ?
 O12 W4 O11 171.8(8) . . ?
 O12 W4 O14 100.4(9) . . ?
 O13 W4 O5 101.9(8) . . ?
 O13 W4 O7 173.2(8) . . ?
 O13 W4 O11 82.7(8) . . ?
 O13 W4 O12 105.4(9) . . ?
 O13 W4 O14 101.3(9) . . ?
 O14 W4 O5 142.8(8) . . ?
 O14 W4 O7 76.8(8) . . ?
 O14 W4 O11 78.4(8) . . ?
 O6 W5 W2 33.0(5) . . ?
 O6 W5 O7 73.0(7) . . ?
 O6 W5 O12 83.4(8) . . ?
 O7 W5 W2 42.1(5) . . ?
 O7 W5 O12 73.4(7) . . ?
 O12 W5 W2 85.6(5) . . ?
 O15 W5 W2 89.3(6) . . ?
 O15 W5 O6 93.8(9) . . ?
 O15 W5 O7 100.8(8) . . ?
 O15 W5 O12 174.1(8) . . ?
 O15 W5 O16 96.7(10) . . ?
 O15 W5 O17 102.3(10) . . ?
 O15 W5 O18 101.8(10) . . ?
 O16 W5 W2 116.2(6) . . ?
 O16 W5 O6 147.2(8) . . ?
 O16 W5 O7 74.6(8) . . ?
 O16 W5 O12 83.1(9) . . ?
 O17 W5 W2 115.2(8) . . ?
 O17 W5 O6 82.4(9) . . ?
 O17 W5 O7 147.1(9) . . ?
 O17 W5 O12 82.5(8) . . ?
 O17 W5 O16 125.0(9) . . ?
 O18 W5 W2 156.7(9) . . ?
 O18 W5 O6 124.7(10) . . ?
 O18 W5 O7 149.8(9) . . ?
 O18 W5 O12 84.0(9) . . ?
 O18 W5 O16 83.1(10) . . ?
 O18 W5 O17 42.7(10) . . ?
 O7 W6 O14 70.8(7) . . ?
 O16 W6 O7 72.0(7) . . ?
 O16 W6 O14 83.1(8) . . ?
 O19 W6 O7 92.5(8) . . ?
 O19 W6 O14 162.2(8) . . ?
 O19 W6 O16 97.4(11) . . ?
 O19 W6 O21 100.8(10) . . ?
 O20 W6 O7 159.1(9) . . ?
 O20 W6 O14 91.8(9) . . ?
 O20 W6 O16 95.2(9) . . ?
 O20 W6 O19 105.8(10) . . ?
 O20 W6 O21 100.2(10) . . ?
 O21 W6 O7 85.9(8) . . ?
 O21 W6 O14 73.0(8) . . ?
 O21 W6 O16 151.8(9) . . ?
 O11 W7 O14 71.4(6) . . ?
 O21 W7 O11 85.5(8) . . ?
 O21 W7 O14 72.0(8) . . ?
 O21 W7 O24 151.2(10) . . ?
 O22 W7 O11 162.1(10) . . ?
 O22 W7 O14 94.5(9) . . ?
 O22 W7 O21 100.9(10) . . ?
 O22 W7 O23 104.0(11) . . ?
 O22 W7 O24 96.7(10) . . ?
 O23 W7 O11 91.7(9) . . ?
 O23 W7 O14 159.8(9) . . ?
 O23 W7 O21 96.4(11) . . ?
 O23 W7 O24 101.3(12) . . ?
 O24 W7 O11 71.4(8) . . ?
 O24 W7 O14 84.1(9) . . ?
 O10 W8 W3 33.6(5) . . ?
 O10 W8 O11 73.6(7) . . ?
 O10 W8 O13 81.4(7) . . ?
 O11 W8 W3 42.7(5) . . ?
 O11 W8 O13 73.5(6) . . ?
 O13 W8 W3 85.7(4) . . ?
 O24 W8 W3 117.9(6) . . ?
 O24 W8 O10 148.0(8) . . ?
 O24 W8 O11 75.6(8) . . ?
 O24 W8 O13 81.9(8) . . ?
 O25 W8 W3 90.7(7) . . ?
 O25 W8 O10 97.3(10) . . ?
 O25 W8 O11 101.8(10) . . ?
 O25 W8 O13 175.3(9) . . ?
 O25 W8 O24 97.2(12) . . ?
 O25 W8 O26 100.0(11) . . ?
 O25 W8 O27 101.2(12) . . ?
 O26 W8 W3 157.3(9) . . ?
 O26 W8 O10 124.3(11) . . ?
 O26 W8 O11 149.5(11) . . ?
 O26 W8 O13 84.4(10) . . ?
 O26 W8 O24 80.7(11) . . ?
 O26 W8 O27 44.2(11) . . ?
 O27 W8 W3 114.3(8) . . ?
 O27 W8 O10 80.7(10) . . ?
 O27 W8 O11 147.3(9) . . ?
 O27 W8 O13 83.1(9) . . ?
 O27 W8 O24 124.0(10) . . ?
 O1 Tb1 K1 44.0(4) . 39_454 ?
 O1 Tb1 O2 80.9(6) . . ?
 O1 Tb1 O3 72.0(6) . 16_545 ?
 O1 Tb1 O8 80.4(6) . . ?
 O1 Tb1 O9 69.0(6) . 39_454 ?
 O1 Tb1 O1W 143.3(7) . . ?
 O1 Tb1 O2W 134.6(6) . . ?
 O1 Tb1 O3W 83.9(7) . . ?
 O1 Tb1 O4W 136.9(7) . . ?
 O2 Tb1 K1 115.5(4) . 39_454 ?
 O2 Tb1 O3 137.9(6) . 16_545 ?
 O2 Tb1 O8 71.4(6) . . ?
 O2 Tb1 O9 73.9(6) . 39_454 ?
 O2 Tb1 O1W 70.8(7) . . ?
 O2 Tb1 O2W 85.9(7) . . ?
 O2 Tb1 O3W 139.5(7) . . ?
 O2 Tb1 O4W 136.5(8) . . ?
 O3 Tb1 K1 63.6(4) 16_545 39_454 ?
 O3 Tb1 O9 122.2(6) 16_545 39_454 ?
 O3 Tb1 O1W 114.9(8) 16_545 . ?
 O3 Tb1 O2W 135.9(7) 16_545 . ?
 O3 Tb1 O3W 69.5(7) 16_545 . ?
 O3 Tb1 O4W 65.2(7) 16_545 . ?
 O8 Tb1 K1 116.2(4) . 39_454 ?
 O8 Tb1 O3 72.7(6) . 16_545 ?
 O8 Tb1 O9 136.6(6) . 39_454 ?
 O8 Tb1 O1W 68.9(7) . . ?
 O8 Tb1 O2W 135.2(7) . . ?
 O8 Tb1 O3W 141.9(7) . . ?
 O8 Tb1 O4W 91.7(8) . . ?
 O9 Tb1 K1 58.7(4) 39_454 39_454 ?
 O9 Tb1 O1W 122.0(8) 39_454 . ?
 O9 Tb1 O2W 65.6(6) 39_454 . ?
 O9 Tb1 O4W 131.6(9) 39_454 . ?
 O1W Tb1 K1 172.6(5) . 39_454 ?
 O2W Tb1 K1 108.3(6) . 39_454 ?
 O2W Tb1 O1W 67.3(8) . . ?
 O2W Tb1 O4W 78.6(8) . . ?
 O3W Tb1 K1 39.9(6) . 39_454 ?
 O3W Tb1 O9 65.5(7) . 39_454 ?
 O3W Tb1 O1W 132.8(8) . . ?
 O3W Tb1 O2W 78.6(8) . . ?
 O3W Tb1 O4W 76.6(9) . . ?
 O4W Tb1 K1 108.0(7) . 39_454 ?
 O4W Tb1 O1W 65.7(9) . . ?
 W1 K1 W3 66.95(12) . . ?
 W1 K1 W3 66.95(12) . 26_554 ?
 W1 K1 Tb1 59.91(11) . 16_545 ?
 W3 K1 W3 133.9(2) . 26_554 ?
 W3 K1 Tb1 97.42(14) 26_554 16_545 ?
 W3 K1 Tb1 58.54(7) . 16_545 ?
 O1 K1 W1 28.3(3) 39_454 . ?
 O1 K1 W1 28.3(3) 16_545 . ?
 O1 K1 W3 58.7(3) 39_454 26_554 ?
 O1 K1 W3 80.2(3) 39_454 . ?
 O1 K1 W3 80.2(3) 16_545 26_554 ?
 O1 K1 W3 58.7(3) 16_545 . ?
 O1 K1 Tb1 88.2(3) 39_454 16_545 ?
 O1 K1 Tb1 31.6(3) 16_545 16_545 ?
 O1 K1 O1 56.6(6) 16_545 39_454 ?
 O4 K1 W1 60.3(4) 26_554 . ?
 O4 K1 W1 60.3(4) . . ?
 O4 K1 W3 121.5(4) . 26_554 ?
 O4 K1 W3 24.4(4) 26_554 26_554 ?
 O4 K1 W3 24.4(4) . . ?
 O4 K1 W3 121.5(4) 26_554 . ?
 O4 K1 Tb1 77.2(4) . 16_545 ?
 O4 K1 Tb1 74.0(4) 26_554 16_545 ?
 O4 K1 O1 65.2(5) 26_554 39_454 ?
 O4 K1 O1 62.9(5) 26_554 16_545 ?
 O4 K1 O1 62.9(5) . 39_454 ?
 O4 K1 O1 65.2(5) . 16_545 ?
 O4 K1 O4 120.5(8) 26_554 . ?
 O4 K1 O21 76.5(6) 26_554 26_554 ?
 O4 K1 O21 162.6(6) 26_554 . ?
 O4 K1 O21 76.5(6) . . ?
 O4 K1 O21 162.6(6) . 26_554 ?
 O4 K1 O3W 92.8(6) . 16_545 ?
 O4 K1 O3W 92.8(6) 26_554 39_454 ?
 O4 K1 O3W 89.6(6) . 39_454 ?
 O4 K1 O3W 89.6(6) 26_554 16_545 ?
 O21 K1 W1 136.6(4) 26_554 . ?
 O21 K1 W1 136.6(4) . . ?
 O21 K1 W3 75.3(4) 26_554 26_554 ?
 O21 K1 W3 145.3(5) . 26_554 ?
 O21 K1 W3 75.3(4) . . ?
 O21 K1 W3 145.3(5) 26_554 . ?
 O21 K1 Tb1 106.5(5) 26_554 16_545 ?
 O21 K1 Tb1 116.3(5) . 16_545 ?
 O21 K1 O1 126.4(5) 26_554 16_545 ?
 O21 K1 O1 133.3(5) . 16_545 ?
 O21 K1 O1 126.4(5) . 39_454 ?
 O21 K1 O1 133.3(5) 26_554 39_454 ?
 O21 K1 O21 86.9(9) 26_554 . ?
 O3W K1 W1 92.4(4) 16_545 . ?
 O3W K1 W1 92.4(4) 39_454 . ?
 O3W K1 W3 68.7(4) 16_545 . ?
 O3W K1 W3 68.7(4) 39_454 26_554 ?
 O3W K1 W3 113.3(4) 39_454 . ?
 O3W K1 W3 113.3(4) 16_545 26_554 ?
 O3W K1 Tb1 152.3(5) 39_454 16_545 ?
 O3W K1 Tb1 32.5(4) 16_545 16_545 ?
 O3W K1 O1 64.1(5) 16_545 16_545 ?
 O3W K1 O1 120.7(6) 16_545 39_454 ?
 O3W K1 O1 120.7(6) 39_454 16_545 ?
 O3W K1 O1 64.1(5) 39_454 39_454 ?
 O3W K1 O21 83.2(6) 16_545 26_554 ?
 O3W K1 O21 83.2(6) 39_454 . ?
 O3W K1 O21 93.3(7) 16_545 . ?
 O3W K1 O21 93.3(7) 39_454 26_554 ?
 O3W K1 O3W 175.2(9) 39_454 16_545 ?
 O17 Na1 O17 117.6(4) 12_554 6 ?
 O17 Na1 O17 117.6(4) 12_554 . ?
 O17 Na1 O17 117.6(4) . 6 ?
 O17 Na1 O18 141.3(6) 12_554 . ?
 O17 Na1 O18 28.2(7) . . ?
 O17 Na1 O18 141.3(6) 6 12_554 ?
 O17 Na1 O18 141.3(6) . 6 ?
 O17 Na1 O18 100.6(6) 6 . ?
 O17 Na1 O18 100.6(6) . 12_554 ?
 O17 Na1 O18 28.2(7) 12_554 12_554 ?
 O17 Na1 O18 28.2(7) 6 6 ?
 O17 Na1 O18 100.6(6) 12_554 6 ?
 O18 Na1 O18 117.0(5) 12_554 . ?
 O18 Na1 O18 117.0(5) 6 . ?
 O18 Na1 O18 117.0(5) 12_554 6 ?
 W1 O1 Tb1 159.6(9) . . ?
 W1 O1 K1 96.0(6) . 39_454 ?
 Tb1 O1 K1 104.4(6) . 39_454 ?
 W2 O2 Tb1 149.2(10) . . ?
 W2 O3 Tb1 154.8(10) . 39_454 ?
 W2 O4 K1 125.3(7) . . ?
 W3 O4 W2 112.9(8) . . ?
 W3 O4 K1 118.9(8) . . ?
 W3 O5 W2 93.4(6) . . ?
 W4 O5 W2 111.0(8) . . ?
 W4 O5 W3 111.8(8) . . ?
 W2 O6 W5 112.8(9) . . ?
 W2 O7 W4 100.7(8) . . ?
 W2 O7 W6 151.8(9) . . ?
 W5 O7 W2 97.7(8) . . ?
 W5 O7 W4 99.2(7) . . ?
 W5 O7 W6 97.1(7) . . ?
 W6 O7 W4 100.3(7) . . ?
 W3 O8 Tb1 147.4(9) . . ?
 W3 O9 Tb1 157.0(10) . 16_545 ?
 W3 O10 W8 111.3(10) . . ?
 W3 O11 W4 100.2(7) . . ?
 W3 O11 W7 153.7(9) . . ?
 W7 O11 W4 99.1(7) . . ?
 W8 O11 W3 97.4(8) . . ?
 W8 O11 W4 99.4(7) . . ?
 W8 O11 W7 96.9(7) . . ?
 W4 O12 W5 105.9(8) . . ?
 W4 O13 W8 104.3(8) . . ?
 W4 O14 W6 111.9(9) . . ?
 W4 O14 W7 110.7(9) . . ?
 W6 O14 W7 92.8(7) . . ?
 W6 O16 W5 111.8(9) . . ?
 W5 O17 Na1 101.2(11) . . ?
 O18 O17 W5 67.3(15) . . ?
 O18 O17 Na1 76.7(15) . . ?
 W5 O18 Na1 101.5(10) . . ?
 O17 O18 W5 70.0(14) . . ?
 O17 O18 Na1 75.1(15) . . ?
 W6 O21 W7 114.9(10) . . ?
 W6 O21 K1 125.0(10) . . ?
 W7 O21 K1 115.9(9) . . ?
 W8 O24 W7 111.7(9) . . ?
 O27 O26 W8 68.0(14) . . ?
 O26 O27 W8 67.8(14) . . ?
 Tb1 O3W K1 107.6(8) . 39_454 ?

_shelx_SHELXL_version_number      '2014/7'
_olex2_submission_special_instructions 'No special instructions were received'

